| Glass acronym | T g (K) | Temperature interval (U c) (K) | Temperature interval (DSC)  (K) | Activation energy ( kJmol -1 ) | Reference and symbol in Fig. 7 |
| ZBL           | 572     | 627-665                        |                                 | 338                            | [6], a                         |
| ZBLALi        | 524     | 600-654                        |                                 | 189                            | [6], b                         |
| ZBLALiPb      | 518     | 603-633                        |                                 | 174                            | [6], c                         |
| ZBL           | 572     |                                | 643-675                         | 315                            | [6], d                         |
| ZBLALi        | 524     |                                | 610-684                         | 168                            | [6], e                         |
| ZBLALiPb      | 518     |                                | 604-661                         | 197                            | [6], f                         |
| ZBLAN20       | 535     | 603-633                        |                                 | 146                            | [7], g                         |
| ZBLAN12       | 546     | 610-628                        |                                 | 292                            | [7], h                         |
| ZBLAN8        | 560     | 603-633                        |                                 | 292                            | [7], i                         |
| ZBLALi        | 529     | 553-594                        |                                 | 337                            | [8], j                         |
| ZBLYAN        | 530     | 593-633                        |                                 | 250                            | [5], m                         |
| ZBLYAN        | 530     | 613-667                        |                                 | 124                            | [5], n                         |
| ZBLYALiPb     | 539     | 568-603                        |                                 | 397                            | This work, o                   |
| ZBLYALiPb     | 539     |                                | 643-693                         | 170                            | This work, p                   |
| ZBLAN         | 530     |                                | 591-602                         | 216                            | [9], q                         |
| ZBLAN         | 530     |                                | 591-602                         | 154                            | [9], r                         |
| ZBA           | 565     |                                | 605-625                         | 497                            | [10]   , s                     |
| ZBALi5        | 549     |                                | 599-619                         | 454                            | [10], t                        |
| ZBALi15       | 529     |                                | 580-606                         | 295                            | [10], u                        |
| ZBALi20       | 524     |                                | 585-610                         | 320                            | [10], v                        |
| ZBALi25       | 513     |                                | 552-563                         | 409                            | [10], w                        |
| ZBALi35       | 493     |                                | 539-559                         | 375                            | [10], x                        |
| ZBGA          | ~610    |                                | 667-684                         | 445                            | [11], y                        |
| ZBLA          | 590     |                                | 631-655                         | 312                            | [12], z                        |

Caption: Glass transition temperatures (T g) and activation energies for crystallisation determined by DSC or from crystal growth rates (U c) in various fluorozirconate glasses

You are provided with a table from a material science paper. Here are JSON templates for two types of numeric cells: "Other" and "Glass_Compound_Amount":
{"value": "xx", "type": "Other"}
{"value": "xx", "type": "Glass_Compound_Amount", "constituent": "xx", "unit": "xx", "material": "xx"}

Please describe all numeric cells in the above table following the JSON templates (proceeding by row in a left-right, top-down direction). For each cell, output one JSON description per line. For any unanswerable attributes in the templates, set their value to the placeholder "xx".

Cell Description:
{"value": "572", "type": "Other"}
{"value": "627", "type": "Other"}
{"value": "665", "type": "Other"}
{"value": "338", "type": "Other"}
{"value": "524", "type": "Other"}
{"value": "600", "type": "Other"}
{"value": "654", "type": "Other"}
{"value": "189", "type": "Other"}
{"value": "518", "type": "Other"}
{"value": "603", "type": "Other"}
{"value": "633", "type": "Other"}
{"value": "174", "type": "Other"}
{"value": "572", "type": "Other"}
{"value": "643", "type": "Other"}
{"value": "675", "type": "Other"}
{"value": "315", "type": "Other"}
{"value": "524", "type": "Other"}
{"value": "610", "type": "Other"}
{"value": "684", "type": "Other"}
{"value": "168", "type": "Other"}
{"value": "518", "type": "Other"}
{"value": "604", "type": "Other"}
{"value": "661", "type": "Other"}
{"value": "197", "type": "Other"}
{"value": "535", "type": "Other"}
{"value": "603", "type": "Other"}
{"value": "633", "type": "Other"}
{"value": "146", "type": "Other"}
{"value": "546", "type": "Other"}
{"value": "610", "type": "Other"}
{"value": "628", "type": "Other"}
{"value": "292", "type": "Other"}
{"value": "560", "type": "Other"}
{"value": "603", "type": "Other"}
{"value": "633", "type": "Other"}
{"value": "292", "type": "Other"}
{"value": "529", "type": "Other"}
{"value": "553", "type": "Other"}
{"value": "594", "type": "Other"}
{"value": "337", "type": "Other"}
{"value": "530", "type": "Other"}
{"value": "593", "type": "Other"}
{"value": "633", "type": "Other"}
{"value": "250", "type": "Other"}
{"value": "530", "type": "Other"}
{"value": "613", "type": "Other"}
{"value": "667", "type": "Other"}
{"value": "124", "type": "Other"}
{"value": "539", "type": "Other"}
{"value": "568", "type": "Other"}
{"value": "603", "type": "Other"}
{"value": "397", "type": "Other"}
{"value": "539", "type": "Other"}
{"value": "643", "type": "Other"}
{"value": "693", "type": "Other"}
{"value": "170", "type": "Other"}
{"value": "530", "type": "Other"}
{"value": "591", "type": "Other"}
{"value": "602", "type": "Other"}
{"value": "216", "type": "Other"}
{"value": "530", "type": "Other"}
{"value": "591", "type": "Other"}
{"value": "602", "type": "Other"}
{"value": "154", "type": "Other"}
{"value": "565", "type": "Other"}
{"value": "605", "type": "Other"}
{"value": "625", "type": "Other"}
{"value": "497", "type": "Other"}
{"value": "549", "type": "Other"}
{"value": "599", "type": "Other"}
{"value": "619", "type": "Other"}
{"value": "454", "type": "Other"}
{"value": "529", "type": "Other"}
{"value": "580", "type": "Other"}
{"value": "606", "type": "Other"}
{"value": "295", "type": "Other"}
{"value": "524", "type": "Other"}
{"value": "585", "type": "Other"}
{"value": "610", "type": "Other"}
{"value": "320", "type": "Other"}
{"value": "513", "type": "Other"}
{"value": "552", "type": "Other"}
{"value": "563", "type": "Other"}
{"value": "409", "type": "Other"}
{"value": "493", "type": "Other"}
{"value": "539", "type": "Other"}
{"value": "559", "type": "Other"}
{"value": "375", "type": "Other"}
{"value": "667", "type": "Other"}
{"value": "684", "type": "Other"}
{"value": "445", "type": "Other"}
{"value": "590", "type": "Other"}
{"value": "631", "type": "Other"}
{"value": "655", "type": "Other"}
{"value": "312", "type": "Other"}